2 downloads
7 Views
2MB Size

Article

Transport Properties of Co in Cu(100) from Density Functional Theory Calculations C. Garcia-Fernandez, Paula Abufager, and Nicolas Lorente J. Phys. Chem. C, Just Accepted Manuscript • DOI: 10.1021/acs.jpcc.7b07661 • Publication Date (Web): 26 Sep 2017 Downloaded from http://pubs.acs.org on September 27, 2017

Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a free service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are accessible to all readers and citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.

The Journal of Physical Chemistry C is published by the American Chemical Society. 1155 Sixteenth Street N.W., Washington, DC 20036 Published by American Chemical Society. Copyright © American Chemical Society. However, no copyright claim is made to original U.S. Government works, or works produced by employees of any Commonwealth realm Crown government in the course of their duties.

Page 1 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

Transport Properties of Co in Cu(100) from Density Functional Theory Calculations. C. García-Fernández,∗,† P. Abufager,‡ and N. Lorente¶ †Donostia International Physics Center (DIPC), Paseo Manuel de Lardizabal 4, 20018 Donostia-San Sebastián,Spain ‡Instituto de Física de Rosario, Consejo Nacional de Investigaciones Científicas y Técnicas (CONICET) and Universidad Nacional de Rosario, Bv. 27 de Febrero 210 bis (2000) Rosario, Argentina ¶Centro de Física de Materiales CFM/MPC (CSIC-UPV/EHU), Paseo Manuel de Lardizabal 5, 20018 Donostia-San Sebastián, Spain E-mail: [email protected]

1 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Abstract The electronic transport properties of a point-contact system formed by a single Co atom adsorbed on Cu (100) and contacted by a copper tip is evaluated in the presence of intra-atomic Coulomb interactions and spin-orbit coupling. The calculations are performed using equilibrium Green’s functions evaluated within density functional theory completed with a Hubbard U term and spin-orbit interaction, as implemented in the Gollum package. We show that the contribution to the transmission between electrodes of spin-flip components is negative and scaling as λ2 /Γ2 where λ is the SOC and Γ the Co atom-electrode coupling. Hence, due to this unfavorable ratio, SOC eﬀects in transport in this system are small. However, we show that the spin-flip transmission component can increase by two orders of magnitude depending on the value of the Hubbard U term. These eﬀects are particularly important in the contact regime because of the prevalence of d-electron transport, while in the tunneling regime, transport is controlled by the sp-electron transmission and results are less dependent on the values of U and SOC. Using our electronic structure and the elastic transmission calculations, we discuss the eﬀect of U and SOC on the well-known Kondo eﬀect of this system.

Introduction The study of single magnetic atoms on non-magnetic metals has become a reality thanks to the advent of local scanning probe microscopies. 1,2 This is a priviledged situation in which precise measurements can be performed on a very controlled environment. Many theoretical works have been recently undertaken to quantitatively evaluate the properties revealed in these experiments. 1–3 Among these properties, Kondo physics 4,5 is currently the object of much interest. 6–13 Here, we take one of these almost-ideal systems and perform calculations to unravel the electronic structure and its eﬀect on the electronic transport revealed by the experiments.

2 ACS Paragon Plus Environment

Page 2 of 24

Page 3 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

The system is a single Co impurity adsorbed on a Cu (100) surface that is contacted by a scanning tunneling microscope (STM) tip. 8,9,11,12 Many interesting eﬀects have been found for this system. Polok and co-workers 14 found that electron transport qualitatively changed with the tip-adatom distance. When the tip was far from the substrate, transport took place through the sp-induced electronic structure of the adatom. When the tip-apex atom approached until reaching covalent-bond distances, the electronic transmission involved the d-system. More curiously, the eﬀect of the tip was a reordering of the electronic structure, changing the system’s properties depending on the tip-surface distance. Unfortunately, these calculations did not address the very interesting Kondo physics experimentally revealed. 11,12 Calculations beyond mean field of Co on Cu (100) showed that dynamical correlation processes were basically controlled by the dz2 orbital of Co. 15–17 Hence, the problem seemed to be greatly simplified by just considering the behavior of the dz2 orbital as the tip-surface distance changed. 18 However, all of these calculations solved Hamiltonians parametrized from plain DFT. A known problem of DFT is its tendency to underestimate the magnetic moments of adsorbed impurities. 19 Particularly, wo important ingredients present in modern calculations were missing from the above studies: the intra-atomic Coulomb interaction as given by the Hubbard U , and the spin-orbit coupling (SOC) of the Co atom. In this work, we consider the mean-field correction of the Hubbard U and the oneelectron spin-orbit coupling both in the tunneling regime that corresponds well to the Co / Cu (100) adsorbed system, and to the contact regime where the tip creates a covalent bond with the Co adatom becoming a point-contact junction. The paper contains a first section devoted to the methodology and setup of the calculations. We first show the results of the electronic structure and transmission calculations for diﬀerent values of the Hubbard U . Next, the paper considers the eﬀect of SOC in the Co atom and its influence on the electronic transmission. We analyze the electron transmission by simplifying the problem to the d-manifold of the Co atom and we rationalize the eﬀect of SOC on the electron

3 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

transmission in terms of the strength of the SOC as compared to electronic coupling the Co d orbitals with the electrodes. We analyze the eﬀects of these modifications in the mean-field electronic structure that serves as basis for parametrized Hamiltonians in the Kondo eﬀect and discuss its influence on previous Kondo studies. 15–18

Computational methodology In this work, we depart from two of the reported optimized geometries of Choi et al. 18 for an atomic junction formed by an adsorbed Co atom on a Cu(100) surface and a copper-covered tip. The two surfaces representing substrate and tip were modeled using a periodic slab geometry with a 3×3 surface unit cell, 6 layers for the surface holding the Co atom and 5 layers for the tip electrode.

Figure 1: Atomic models with the two configurations used along this work:(a) the tunneling regime where the distance between the Co atom and the tip apex is 5.05 Å and (b) the contact regime where the same distance diminishes until typical covalent-bonding distances, here 2.2 Å. Periodic boundary conditions have been applied along the axes perpendicular to the transport direction. Along this last one, open-boundary conditions proper to the transport problem are applied. DFT calculations have been performed within the spin-polarized generalized gradient approximation (GGA-PBE). 20 Troullier-Martins full-relativistic pseudo-potentials, 21 an energy cutoﬀ of 500 Ry and a 7×7×3 K-point mesh generated according to the Monkhorst-Pack scheme, have been used in the Siesta code. 22 A double-ζ plus polarization (DZP) basis set 4 ACS Paragon Plus Environment

Page 4 of 24

Page 5 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

was defined to describe the Co and surface-atom electrons, while diﬀuse orbitals were used to improve the surface electronic description. Furthermore, a single-ζ plus polarization (SZP) basis was set for the copper electrodes. Note that we employ a DZP basis set to describe the adsorbate states in order to yield correct transmission functions. 23 Quantum transport computations were performed from DFT within the framework of the Landauer-Buttiker formalism. Thus, the DFT Hamiltonian and overlap matrices obtained with Siesta 22 were analized in a post-processing step with the Gollum package. 24 This code is based on equilibrium transport theory and by carefully setting electrodes, branches and the central scattering region, 25 the transmision coeﬃcients can be computed without performing independent selfconsistent calculations of the density matrix. This approach results in considerable savings of time and computational resources. Furthermore, one of the attractive features of Gollum is its functionality to compute spin transport in systems with spin-orbit interactions. Comparison with previous calculations 18 using self-consistent non-equilibrium Green’s function calculations shows that both calculations agree within the available numerical precision.

Results and discussion Electronic structure and transport The goal of the present section is to explore the sensitivity of the electronic and transport properties of the Cu-Co-Cu junction with respect to two distinct interactions: the Coulomb on-site repulsion, or Hubbard U , on Co-d orbitals and the spin-orbit coupling (SOC). We first analize the eﬀect of the U parameter on the electronic and transport properties of the system comparing with the results of standard DFT (for the PBE exchange-andcorrelation functional) in the tunnel Fig. 2 and contact regimes Fig. 3. Next, we include spin-orbit coupling and evaluate the same properties. We simplify the calculations to include just the d-electrons of the Co atom and rationalize our findings at the end of this section. 5 ACS Paragon Plus Environment

The Journal of Physical Chemistry

-1

4

10

Ueff=0

Ueff=0

2

10 0 -2 -4

T

PDOS

-2

dxy dx2-y2 dz2 dxz dyz

-3

10

(a)

(b)

-4

-3

-2

-1

0

1

2

10 -2

3

-1

E-EFermi(eV)

0

1

2

E-EFermi(eV) -1

4

10

Ueff=3 eV

Ueff=3 eV

2

-2

10 0 -2 -4

T

PDOS

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Page 6 of 24

dxy dx2-y2 dz2 dxz dyz

-3

10

(d)

(c) -4

-3

-2

-1

0

1

2

10 -2

3

E-EFermi(eV)

-1

0

1

2

E-EFermi(eV)

Figure 2: Results in the tunneling configuration for: (a,c) Density of states projected onto Co-d atomic orbitals (PDOS) and (b,d) electron transmissions T between electrodes as a function of electron energy referred to the Fermi energy (E −EF ermi ). No spin-orbit coupling is included and the graphs are divided in majority (positive PDOS and up arrow for T) and minority (negative PDOS and down arrow for T) spins. The Hubbard-U of the Co d-manifold used in the GGA+U scheme are Uef f = 0 eV in the upper graphs (a,b), and Uef f = 3 eV in the lower ones, (c,d).

Eﬀect of U on the electronic and transport properties Fig. 2(a) and 3(a) shows the PDOS projected onto Co-d atomic orbitals, computed in this study without the inclusion of the Coulomb on-site repulsion, in the tunneling and contact configurations respectively. When the tip is far from the cobalt atom (fig. 2(a)), the two singly occupied dz2 ,dx2 −y2 magnetic orbitals are clearly shown as unoccupied states, in good agreement with the results by Polok et al. 14 and Baruselli et al. 15 However, the detailed electronic structure of the Co adatom changes in the contact region (fig. 3(a)). There is a re-ordering of the minority spin d-states and contributions from dz2 , dxz

6 ACS Paragon Plus Environment

Page 7 of 24

1

4

10

Ueff=0

Ueff=0 T

PDOS

2

0

-2

-4 -3

dxy dx2-y2 dz2 dxz dyz

0

10

(a)

(b) -1

-2

-1

0

1

2

10 -2

3

-1

E-EFermi(eV)

2

10

Ueff=3 eV T

0

-4 -3

1

E-EFermi(eV)

Ueff=3 eV

2

-2

0

1

4

PDOS

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

dxy dx2-y2 dz2 dxz dyz

-2

0

10

(c)

(d) -1

-1

0

1

2

10 -2

3

E-EFermi(eV)

-1

0

1

2

E-EFermi(eV)

Figure 3: Results in the contact configurations for: (a,c) PDOS and (b,d) electron transmissions T with the same parameters and conventions as in Fig. 2.The transmission T trough the majority (minority) spin channels at the Fermi level are 1.73 (2.66) for Uef f = 0 and 1.65 (2.25) for Uef f = 3, respectively. and dyz orbitals become important at the Fermi level. 14,18 In spite of the changes observed in the electronic structure, the overall magnetic properties slightly change since the Co adatom can be described as in a 3d8 (S = 1) configuration in both regimes. 14–18,26 The re-ordering of d levels in contact induces changes in the transport properties, as was previously reported. 14,18 In the tunneling region, we find that transport Fig. 2 (b) basically takes place through the majority spin sp electrons of the Co atom. In the contact regime, however, the d-electron contribution to the transmission at the Fermi level for the minority spin highly increases and the transport is governed by the minority spin channel. Indeed, the spin polarization defined as P = (T↑ (EF ) − T↓ (EF ))/(T↑ (EF ) + T↓ (EF )), where Tσ (EF ) is the transmission per spin σ at the Fermi energy, changes its sign when going from tunneling to contact.

7 ACS Paragon Plus Environment

The Journal of Physical Chemistry

As reported before, 14,18 our present calculations confirm the previous picture where conduction takes place through the sp electrons of the Co adatom in tunneling while Co d-orbitals dominate the transport in the contact regime. The Coulomb on-site repulsion on Co d-orbitals is an indispensable component in the above scenario. Since such interaction could modify the picture if the partially occupied dz2 , dxz and dyz orbitals are pulled down with respect to unoccupied orbitals when U is increased. Here, we explore such an issue by performing LDA+U calculations through the simplified rotationally invariant formulation of Dudarev et al, 27 with an eﬀective Uef f = U − J that includes the eﬀect of the Fock exchange interaction, J. We use the implementation of the Siesta code. 28 6 Ueff= 0 eV

4

PDOS

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Page 8 of 24

Ueff= 3 eV

2

Ueff= 4 eV

0 -2 -4 -3

-2

-1

0

1

2

3

E-EFermi(eV) Figure 4: Spin-polarized PDOS projected onto Co(3d) atomic orbitals at contact for Uef f = U − J = 0, 3, 4 eV As depicted in Fig. 2(c) (Uef f = 3 eV) the overall properties for the tunnel regime slightly change with respect to the PDOS computed at the DFT level (Fig. 2(a)), being the main quantitative feature related to an increase of the energy separation among dlevels. However, when the tip is close to the surface, Fig. 3(c), the minority dz2 is shifted to lower energies, leaving the dxz and dyz as the only orbital contributions around the Fermi energy. The increase of the separation among levels and the decrease of the minority channel contribution at the Fermi energy when including the Coulomb repulsion can be clearly seen in Fig. 4 depicting the total Co 3d PDOS for three diﬀerent values of the eﬀective Uef f .

8 ACS Paragon Plus Environment

Page 9 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

It is instructive to compare these results with finite-size calculations using complete active space self-consistent field (CASSCF). 29–31 The occupation of the d-electron manifold is virtually identical for the CASSCF results and the DFT results in tunneling. The reported values 31 are 2.0 electrons in the dx2 −y2 , dxz and dyz orbitals and 1.0 electron in the dz2 and dxy . The above Uef f = 0 results are 2.0, 1.8 and 1.1 respectively. For Uef f = 3 eV these results are even closer to CASSCF calculations (note the trivial rotation from dx2 −y2 to dxy between calculations). Despite this resemblance, the final electronic structure can qualitatively diﬀer as can be seen in the above Uef f = 0 and Uef f = 3 eV results plotted in Figs.2 (a) and (c). In transport, a large Co sp contribution remains in the transmission at the Fermi level. As a result, good agreement is found between Uef f = 0 eV and Uef f = 3 eV calculations as can be seen from Figs.

2 (b) and (d). When the tip is near the surface adatom, two

diﬀerences are clearly seen between Uef f = 3 eV (Fig. 3(d)) and Uef f = 0 eV (Fig. 3(b)). There is a shift in the energy scale, related to the new energy position of the Co orbitals. The second diﬀerence is a decrease of 4% and 15% of T (EF ) with respect to the Uef f = 0 values computed for the majority and minority spin channels, respectively. This diﬀerence can be traced back to a change in the dz2 orbital energy. In spite of these diﬀerences, the overall scenario of Refs. 14,18 based on the leading transmission through the minority spin channel governed by Co-d orbitals remains unchanged. Therefore, we can conclude that the Coulomb on-site repulsion on Co-d orbitals does not have a strong eﬀect on the transport properties of the Co junction.

Electronic transport in the presence of spin-orbit coupling We include spin-orbit coupling (SOC) in the DFT equations following the implementations in Siesta 22 and Gollum. 24 The PDOS, Fig. 5 (a) (Uef f = 0), reveals that the eﬀect of SOC on the electronic structure of the Co-adatom is negligible within the accuracy of DFT calculations. This translates into the calculations of the electron transmission, showing that the presence of SOC produces no eﬀect. Figure 5(b) compares the transmission with and 9 ACS Paragon Plus Environment

The Journal of Physical Chemistry

without SOC. Both curves agree. However, the plotted total transmission is the sum of four terms. Mainly the direct non-spin-flip transmissions and the transmissions where the electron spin changes between electrodes. In the next section, we study the spin-flip contributions to the transmission and their sensibility to the Coulomb on-site repulsion. 6

PDOS

4 2 0 -2

(a)

-4 -2

-1

0

1

2

E-EFermi(eV) 1

10

T

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Page 10 of 24

(b) 0

10 -2

-1

0

1

2

E-EFermi(eV) Figure 5: Total (a) PDOS projected onto Co(3d) atomic orbitals and (b) transmission at contact with (orange line) and without (black line) taking into account spin-orbit interactions and Uef f = 0.

Spin-orbit assisted spin-flip scattering The present problem consists in a single center where the SOC is localized. We use the electronic structure computed above (with and without the inclusion of Uef f ) to compute the transmission by just considering the transmission through the d-orbitals that are the ones containing sizeable SOC contributions. This approximation is particularly well fitted to the contact regime. In Ref. 18 three channels of strong d character are shown to dominate the

10 ACS Paragon Plus Environment

Page 11 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

transmission at contact while the sp channels dominate transport in the tunneling regime. The transmission between electrodes for an electron injected at energy E through the d-orbitals of the Co atoms is:

T (E) =

∑

a ΓLi,j Grj,k ΓR k,l Gl,i .

(1)

i,j,k,l

Where i, j, k, l are indices over the spin orbitals of the d-electron manifold. The Green’s functions Grj,k and Gal,i are the retarded and advance resolvents of the atomic Hamiltonian, ˆ in contact with the two electrodes, expressed again in the d-electron spin orbitals: H, r(a) ˆ −Σ ˆ r(a) ]−1 |j⟩. Gj,k = ⟨i|[E ˆ1 − H

(2)

The identity operator, ˆ1, becomes a matrix of the dimension of the d manifold as well as ˆ r(a) . The imaginary part of the self-energy is actually the retarded (advanced) self-energy, Σ related to Γ of each electrode by (here i is the imaginary unit):

ˆ = iΣ ˆ r − iΣ ˆ a. Γ

(3)

The total self-energy is the sum of self-energies due to each electrode. In the spirit of the above calculations, we use Kohn-Sham orbitals, and the problem becomes a one-electron transport problem. From this analysis we find that for E between −2 and 2 eV transport at contact is dominated by three d orbitals in good agreement with previous results, Ref. 18 Prior to switching on the SOC, we can identify the three spin orbitals as the minority spin degenerated dxz and dyz with some further contribution from the dz2 orbital. This is particularly true for the Uef f = 0 cases, Figures 3 (a) and (b). The minority spin peak that dominates the transmission at the Fermi energy is clearly a contribution of the just mentioned orbitals. However, for Uef f = 3 eV, the dz2 orbital shifts down in energy and the transmission at the Fermi energy is controlled by the minority-spin degenerated dxz

11 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Page 12 of 24

and dyz . The comparison of Figs. 3 (a) and (c) show the clear reduction of the weight of dz2 -type electronic structure at the Fermi energy. This is concomitant with the appearance of a sharp minimum at ∼ −1.5 eV in Fig. 3 (d). Our calculations using the transmission through d orbitals, Eq. (1), show that its origin is a sizeable interference term Γz2 ,xy due to the mixing of orbitals by the Cu d-band that starts at ∼ −1.8 eV. ˆ restricted to the d-electron subspace. This is The SOC is included in Hamiltonian, H, particularly simple to do in the Cartesian representation of d electrons. We follow Ref., 32 where all matrix elements are carefully written. We write the SOC contribution to the Hamiltonian as:

ˆ SOC = λ(L ˆ z Sˆz + L ˆ x Sˆx + L ˆ y Sˆy ) H ˆ z Sˆz + 1 [L ˆ + Sˆ− + L ˆ − Sˆ+ ]). = λ(L 2

(4)

While the first term connects orbitals with the same |m| and spin, where m is the eigenvalue ˆ z , the second term leads to spin-flips connecting spin-orbitals with diﬀerent spins and of L orbitals of |m ± 1|. If we consider the matrix elements in Cartesian terms, we also remark ˆ z Sˆz and L ˆ x Sˆx are purely imaginary, L ˆ y Sˆy are purely that while the matrix elements of L real. All diagonal matrix elements are zero because in Cartesian orbitals the average angular momentum is zero.

It is straightforward to build the new Green’s function by inverting the old Hamiltonian with the above additional term, Eq. (4). The value we took for λ was the one of Co (I) because DFT yields a 3d8 state for Co (S = 1) in the contact configuration. 18 Using the values of Ref. 33 we have that ⟨ξ⟩ = 455 cm−1 , and

λ=

⟨ξ⟩ = 0.0284 eV. 2S

12 ACS Paragon Plus Environment

(5)

2 0 -2 -4

-3

T (x10 )

-2

-5

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

T (x10 )

Page 13 of 24

0

(a)

-4

-2

(b) -1

0

1

2

E-EFermi(eV)

Figure 6: Spin-flip component of the transmission for (a) Uef f = 0 and (b) Uef f = 3 eV in the Co d-manifold. There is a factor-of-100 diﬀerence in the transmission between (a) and (b) marked in the y-axis label. We retrieve our calculations using DFT with SOC for the transmission function, Fig. 5 (b), with the message that λ is so small that the eﬀect on the transmission is negligible. As we will show in the next section, SOC eﬀects will be noticeable as soon as the ratio (λ/Γ)2 is not small, where Γ is the width of the d levels given by Eq. (3). Since the spin of the electron in the electrodes is a good quantum number, we can study the transmission of each spin. From Eq. (1), we single out the spins and follow the transmission of each spin. We see that the transmission is a 2 × 2 matrix in spin due to the combinations of entering with either up or down spins and exiting with up and down including cross terms where the spin flips due to the presence of SOC at the Co atom. Let us analyze the spin-flip term:

a T↑,↓ (E) = T r[ΓL↑ Gr↑,↓ ΓR ↓ G↓,↑ ].

(6)

T r stands for trace over d orbitals and there are three matrix products because both Γ’s and G’s are matrices on d orbitals. Figure 6 shows the results for the spin-flip transmission, T↑,↓ (E) of Eq. (6). This contribution is negative, leading to the decrease of electron transmission in the system and to the increase of electron backscattering. Despite their small value stemming from the small-

13 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Page 14 of 24

ness of λ/Γ, we see fundamental diﬀerences between the two plotted cases. Figure 6(a) is the Uef f = 0 case while Fig. 6(b) is the Uef f = 3 eV one. The diﬀerence of two orders of magnitude between the two cases comes from the diﬀerent electronic structure. In the Uef f = 0 case, the three orbitals dz2 , dxz and dyz are close in energy about the Fermi level. These three orbitals have non-zero spin-orbit matrix elements connecting them because of the above spin-flip rule. Namely, the flipping of an electron leads to the change of |m| where m is the third component of the angular momentum of the spherical harmonics entering the orbital. Spin-flip then involves matrix elements changing |m| by one, which is the case between the degenerated dxz and dyz with the m = 0, dz2 orbital. When Uef f = 3 eV, the dz2 orbital moves by more than 1.5 eV away from the dxz and dyz orbitals, quenching the spin-flip probabilities.

Simplified spin-orbit transmission It is interesting to simplify the above treatment to enhance our insight into the spin-orbitinduced spin flip. Let us assume a single d orbital. In this case the spin-orbit contribution to the Hamiltonian becomes: 34 ˆ SOC = iλ(dˆ† dˆ↓ − dˆ† dˆ↑ ). H ↓ ↑

(7)

This is obviously Hermitian, and the matrix element is iλ, purely imaginary. We adopt the broken-symmetry description of DFT, then, the atomic level becomes ϵ↑ and ϵ↓ = ϵ↑ + U with U the Hubbard charging energy. Within the wide-band approximation, the Green’s function of the orbital in contact with two electrodes is: −1 R ΓL ↑ +Γ↑ −iλ E − ϵ↑ + i 2 G(E) = R ΓL ↓ +Γ↓ iλ E − ϵ↓ + i 2

(8)

with obvious notations for the self-energies of the level due to the left and right electrodes 14 ACS Paragon Plus Environment

Page 15 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

(real parts are strictly zero in the wide-band approximation) for each spin. Replacing these quantities in Eq. (1), we obtain for the direct terms:

T↑,↑ (E) =

R ΓL ↓ +Γ↓ 2 | 2 L Γ +ΓR ϵ↓ + i ↓ 2 ↓ )

ΓL↑ ΓR ↑ |E − ϵ↓ + i |(E − ϵ↑ +

ΓL +ΓR i ↑ 2 ↑ )(E

−

−

(9)

λ2 |2

In the limit λ → 0 we retrieve the usual result:

T↑,↑ (E) =

ΓL↑ ΓR ↑ |E − ϵ↑ + i

R ΓL ↑ +Γ↑ 2 | 2

(10)

.

The spin-flip term is proportional to λ2 :

T↑,↓ (E) =

2 ΓL↑ ΓR ↓ (iλ)

|(E − ϵ↑ + i

R ΓL ↑ +Γ↑ )(E 2

− ϵ↓ + i

R ΓL ↓ +Γ↓ ) 2

− λ2 |2

.

(11)

In the limit of large ΓR ∼ ΓL ∼ Γ ≫ ϵ↑ we see that the spin-flip contribution to the transmission becomes a negative quantity quadratic on the λ to Γ ratio:

T↑,↓ (E) ∼ −

λ2 . Γ2

(12)

This sets a scale for the values of λ that yield sizeable spin-flip terms in electron transport. Typically Γ is about a few hundred meV. If λ is in the tens of meV (3d transition metals) the spin-flip terms will be negligible in transport for a single scattering center. However, heavy elements will produce important spin-flips in point contacts.

Kondo eﬀect The computed electronic structure has direct bearings on the Kondo eﬀect that a Co impurity displays in contact with copper electrodes. 15–17 The very diﬀerent electronic properties of the calculations of Figs. 2 (a) and (c) depending on the value of the Hubbard U , will change the interpretation of this Kondo eﬀect. Indeed, for Uef f = 0, Fig. 2 (a) is in perfect agreement 15 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

with the analyses published in Refs., 15–17 leading to the conclusion that the S=1 Kondo eﬀect is actually a two-stage Kondo, where initially a S=1/2 Kondo eﬀect is produced by the dz2 -orbital charge fluctuations and the remaining magnetic moment gets screened at lower temperatures, driven by the charge fluctuations of the dx2 −y2 orbital. The above picture is qualitatively the same as U increases, Fig. 2 (c). Although the quantitative details will strongly vary. This is in agreement with the discussion by Baruselli et al. 15 on the values of the computed Kondo temperatures pointing out the many diﬃculties to estimate accurate values based on DFT calculations. At contact the picture radically changes. Figures 3 (a) and (c) show the half-occupied dx2 −y2 orbital leads to a S=1/2 Kondo eﬀect. The dz2 orbital is not relevant for Kondo physics anymore because it becomes completely occupied. The rest of the magnetic moment is screened by the charge fluctuations of a mixed-valence regime driven by the degenerate dxz and dyx orbitals. Qualitatively, the inclusion of U does not change the discussion although the final values will greatly diﬀer. The above results show that the Kondo eﬀect of Co in contact with Cu electrodes can be considered as a single-orbital Kondo eﬀect, at least for a large range of temperatures in the tunneling regime, and probably for all temperatures at contact. In this last case, nonequilibrium eﬀects have been discussed before. 18 The main eﬀect at contact is the increased coupling to the electrodes given by Γ. The intrinsically non-equilibrium eﬀects (bias-induced decoherence and peak splitting) are largely absent from the conductance behavior in the contact regime. 18 The eﬀect of spin-orbit interactions in Kondo processes has been much debated in the literature. Most works refer to the influence of a Rashba-like spin-orbit interaction on the Kondo spin-flip processes. The debate was very much calmed by the work of Meir and Wingreen 35 showing that due to the preservation of time-reversal symmetry by the spin-orbit interaction, Kramers degeneracy is maintained and the Kondo processes are not aﬀected. Recent works actually show that Rashba eﬀects can change the Kondo temperature reducing

16 ACS Paragon Plus Environment

Page 16 of 24

Page 17 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

it 36,37 or increasing it 38 depending on the system. Indeed, the eﬀect of the environment is very important. Újsághy and co-workers 39,40 showed that SOC can lead to sizeable magnetic anisotropies depending on the environment. This has important consequences for local spins larger than 1/2, because it reduces the spin degeneracy and prevents Kondo spin-flip processes. Here, we are considering the local SOC of a single impurity and not the extended Rashba-like interactions. Since the mean-field spin of cobalt is close to 1, we expect to find the disruptions caused by an emerging anisotropy due to SOC and the environment of the Co atom. However, our calculation yields a very small magnetic anisotropy energy (MAE) when a Co atom is adsorbed on the Cu (100) surface. The MAE is ∼ 2 meV. Dividing by the Boltzmann constant yields a MAE ∼ 23 K much smaller than TK ∼ 90 K, the Kondo temperature of Co on Cu (100). 11,12,41 Hence, we do not expect any eﬀect of the SOC in the tunneling regime. When the tip contacts the impurity, we find that the symmetry of the environment of the Co atom increases, further reducing the MAE to ∼ 0.03 meV and unaﬀecting the Kondo physics.

Conclusions Electron transport through a Co atom between an STM tip and a Cu (100) substrate is shown to be largely independent of the Hubbard U values used in the evaluation of the electronic structure. Despite the dramatic eﬀects of the inclusion of U , transport at the Fermi energy is basically controlled by the same orbitals. When the tip is far from the substrate, the tunneling regime is led by cobalt’s sp-electronic structure. At contact, the d-electronic structure controls all electronic transport properties. Surprisingly, the electronic transmission with or without Hubbard U for both transport regimes is qualitatively the same and to a large extent also quantitatively. The inclusion of spin-orbit coupling (SOC) does not change the quantitative values of transmission. We show that this is due to the small λ/Γ ratio, where λ is the SOC values

17 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

and Γ is the Co electronic coupling to the electrodes. Transport with spin-orbit interactions gives rise to spin-flip processes. At lowest-order in the above ratio we find that the spin-flip component of the transmission is T↑,↓ (E) ∼ −λ2 /Γ2 . Hence, for Co in metals this value is very small, but for heavier impurities, it will lead to sizeable decreases of electron transmission. The eﬀect of the Hubbard U in the spin-orbit induced spin-flip transmission is dramatic. This is due to the shifting of critical orbitals to be able to complete a spin-flip process. Indeed the non-zero matrix elements of the SOC involve ∆Sz = ±1 and ∆m = ±1 states, where Sz and m correspond to the spin and orbital-angular moment. When the values of Uef f are ramped from zero to 3 eV, the ∆m = ±1 states eﬀectively split, reducing in two orders of magnitude the spin-flip component of the electron transmission, T↑,↓ . The Kondo eﬀect is strongly aﬀected by the values of the Hubbard U although the qualitative picture gleaned in previous works 15–18 remains unchanged. Moreover, we find that the Co SOC leads to small magnetic anisotropy energies, well below the typical Kondo temperatures, bearing no eﬀect on Kondo processes for any of the conductance regimes analyzed here. Hence, calculations based on DFT parametrizations should be qualitatively correct in describing the Kondo eﬀect, particularly for the case of Co atomic impurities. We further show that the absence of spin-orbit coupling is justified besides the comparable Kondo and spin-orbit energy scales.

Acknowledgement We thank Jaime Ferrer, Pablo Rivero and Salva Barraza for providing us with their cobalt pseudopotential. We further thank Jaime Ferrer for providing us with a copy of Gollum and for instructing us on its use. We thank Roberto Robles for many discussions and ideas. We gratefully acknowledge support from MINECO (Grant No. MAT2015-66888-C3-2-R), FEDER funds, the CCT-Rosario Computational Center and CONICET.

18 ACS Paragon Plus Environment

Page 18 of 24

Page 19 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

References (1) Gauyacq, J.-P.; Lorente, N.; Novaes, F. D. Excitation of local magnetic moments by tunneling electrons. Progress in Surface Science 2012, 87, 63 – 107. (2) Ternes, M. Probing magnetic excitations and correlations in single and coupled spin systems with scanning tunneling spectroscopy. Progress in Surface Science 2017, 92, 83 – 115. (3) Delgado, F.; Fernández-Rossier, J. Spin decoherence of magnetic atoms on surfaces. Progress in Surface Science 2017, 92, 40 – 82. (4) Kondo, J. Resistance minimum in dilute magnetic alloys. Progress of Theoretical Physics 1964, 32, 37–49. (5) Hewson, A. C. The Kondo Problem to Heavy Fermions; Cambridge studies in magnetism; Cambridge University Press, 1993. (6) Li, J.; Schneider, W.-D.; Berndt, R.; Delley, B. Kondo scattering observed at a single magnetic impurity. Phys. Rev. Lett. 1998, 80, 2893–2896. (7) Madhavan, V.; Chen, W.; Jamneala, T.; Crommie, M. F.; Wingreen, N. S. Tunneling into a single magnetic atom: Spectroscopic evidence of the Kondo resonance. Science 1998, 280, 567–569. (8) Knorr, N.; Schneider, M. A.; Diekhöner, L.; Wahl, P.; Kern, K. Kondo eﬀect of single Co adatoms on Cu surfaces. Phys. Rev. Lett. 2002, 88, 096804. (9) Néel, N.; Kröger, J.; Limot, L.; Palotas, K.; Hofer, W. A.; Berndt, R. Conductance and Kondo eﬀect in a controlled single-atom contact. Phys. Rev. Lett. 2007, 98, 016801. (10) Ternes, M.; Heinrich, A. J.; Schneider, W.-D. Spectroscopic manifestations of the Kondo eﬀect on single adatoms. Journal of Physics: Condensed Matter 2009, 21, 053001. 19 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

(11) Vitali, L.; Ohmann, R.; Stepanow, S.; Gambardella, P.; Tao, K.; Huang, R.; Stepanyuk, V. S.; Bruno, P.; Kern, K. Kondo eﬀect in single atom contacts: The importance of the atomic geometry. Phys. Rev. Lett. 2008, 101, 216802. (12) Choi, D.-J.; Rastei, M. V.; Simon, P.; Limot, L. Conductance-driven change of the Kondo eﬀect in a single Cobalt atom. Phys. Rev. Lett. 2012, 108, 266803. (13) Choi, D.-J.; Guissart, S.; Ormaza, M.; Bachellier, N.; Bengone, O.; Simon, P.; Limot, L. Kondo resonance of a Co atom exchange coupled to a ferromagnetic tip. Nano Letters 2016, 16, 6298–6302. (14) Polok, M.; Fedorov, D. V.; Bagrets, A.; Zahn, P.; Mertig, I. Evaluation of conduction eigenchannels of an adatom probed by an STM tip. Phys. Rev. B 2011, 83, 245426. (15) Baruselli, P. P.; Requist, R.; Smogunov, A.; Fabrizio, M.; Tosatti, E. Co adatoms on Cu surfaces: Ballistic conductance and Kondo temperature. Phys. Rev. B 2015, 92, 045119. (16) Jacob, D. Towards a full ab initio theory of strong electronic correlations in nanoscale devices. Journal of Physics: Condensed Matter 2015, 27, 245606. (17) Frank, S.; Jacob, D. Orbital signatures of Fano-Kondo line shapes in STM adatom spectroscopy. Phys. Rev. B 2015, 92, 235127. (18) Choi, D.-J.; Abufager, P.; Limot, L.; Lorente, N. From tunneling to contact in a magnetic atom: The non-equilibrium Kondo eﬀect. The Journal of Chemical Physics 2017, 146, 092309. (19) Anisimov, V. I.; Aryasetiawan, F.; Lichtenstein, A. I. First-principles calculations of the electronic structure and spectra of strongly correlated systems: the LDA + U method. Journal of Physics: Condensed Matter 1997, 9, 767–808.

20 ACS Paragon Plus Environment

Page 20 of 24

Page 21 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

(20) Perdew, J. P.; Burke, K.; Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 1996, 77, 3865–3868. (21) Troullier, N.; Martins, J. L. Eﬃcient pseudopotentials for plane-wave calculations. Phys. Rev. B 1991, 43, 1993. (22) Soler, J. M.; Artacho, E.; Gale, J. D.; García, A.; Junquera, J.; Ordejón, P.; SánchezPortal, D. The SIESTA method for ab initio order- N materials simulation. Journal of Physics: Condensed Matter 2002, 14, 2745. (23) Abufager, P. N.; Robles, R.; Lorente, N. FeCoCp3 molecular magnets as spin filters. The Journal of Physical Chemistry C 2015, 119, 12119–12129. (24) Ferrer, J.; Lambert, C. J.; GarcÃŋa-Suárez, V. M.; Manrique, D. Z.; Visontai, D.; Oroszlany, L.; Rodríguez-Ferradás, R.; Grace, I.; Bailey, S. W. D.; Gillemot, K. et al. GOLLUM: a next-generation simulation tool for electron, thermal and spin transport. New Journal of Physics 2014, 16, 093029. (25) GOLLUM 1.1: User Manual. GOLLUM 1.1: User Manual 2015, , . (26) Surer, B.; Troyer, M.; Werner, P.; Wehling, T. O.; Läuchli, A. M.; Wilhelm, A.; Lichtenstein, A. I. Multiorbital Kondo physics of Co in Cu hosts. Phys. Rev. B 2012, 85, 085114. (27) Dudarev, S. L.; Botton, G. A.; Savrasov, S. Y.; Humphreys, C. J.; Sutton, A. P. Electron-energy-loss spectra and the structural stability of nickel oxide:âĂĆâĂĆAn LSDA+U study. Physical Review B 1998, 57, 1505. (28) Wierzbowska, M.; Sánchez-Portal, D.; Sanvito, S. Diﬀerent origins of the ferromagnetic order in (Ga,Mn)As and (Ga,Mn)N. Phys. Rev. B 2004, 70, 235209. (29) Huang, P.; Carter, E. A. Local electronic structure around a single Kondo impurity. Nano Letters 2006, 6, 1146–1150. 21 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

(30) Huang, P.; Carter, E. A. Ab initio explanation of tunneling line shapes for the Kondo impurity state. Nano Letters 2008, 8, 1265–1269. (31) Sharifzadeh, S.; Huang, P.; Carter, E. A. Origin of tunneling lineshape trends for Kondo states of Co adatoms on coinage metal surfaces. Journal of Physics: Condensed Matter 2009, 21, 355501. (32) Dai, D.; Xiang, H.; Whangbo, M.-H. Eﬀects of spin-orbit coupling on magnetic properties of discrete and extended magnetic systems. Journal of Computational Chemistry 2008, 29, 2187–2209. (33) Dai, D.; Whangbo, M.-H. Analysis of the uniaxial magnetic properties of high-spin d6 ions at trigonal prism and linear two-coordinate sites: Uniaxial magnetic properties of Ca3Co2O6 and Fe[C(SiMe3)3]2. Inorganic Chemistry 2005, 44, 4407–4414. (34) Wilhelm, J.; Walz, M.; Evers, F. Ab initio. Phys. Rev. B 2015, 92, 014405. (35) Meir, Y.; Wingreen, N. S. Spin-orbit scattering and the Kondo eﬀect. Phys. Rev. B 1994, 50, 4947–4950. (36) Žitko, R.; Bonča, J. Kondo eﬀect in the presence of Rashba spin-orbit interaction. Phys. Rev. B 2011, 84, 193411. (37) Yanagisawa, T. Kondo eﬀect in the presence of spinâĂŞorbit coupling. Journal of the Physical Society of Japan 2012, 81, 094713. (38) Zarea, M.; Ulloa, S. E.; Sandler, N. Enhancement of the Kondo eﬀect through Rashba spin-orbit interactions. Phys. Rev. Lett. 2012, 108, 046601. (39) Újsághy, O.; Zawadowski, A.; Gyorﬀy, B. L. Spin-orbit-induced magnetic anisotropy for impurities in metallic samples of reduced dimensions: Finite size dependence in the Kondo eﬀect. Phys. Rev. Lett. 1996, 76, 2378–2381.

22 ACS Paragon Plus Environment

Page 22 of 24

Page 23 of 24

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

The Journal of Physical Chemistry

(40) Újsághy, O.; Zawadowski, A. Spin-orbit-induced magnetic anisotropy for impurities in metallic samples. II. Finite-size dependence in the Kondo resistivity. Phys. Rev. B 1998, 57, 11609–11622. (41) Néel, N.; Kröger, J.; Limot, L.; Palotas, K.; Hofer, W. A.; Berndt, R. Conductance and Kondo eﬀect in a controlled single-atom contact. Phys. Rev. Lett. 2007, 98, 016801.

23 ACS Paragon Plus Environment

The Journal of Physical Chemistry

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 43 44 45 46 47 48 49 50 51 52 53 54 55 56 57 58 59 60

Graphical TOC Entry

24 ACS Paragon Plus Environment

Page 24 of 24